Numerical Modeling of Delamination Resistance Improvement Through The Use of CNTReinforced Bonding Layers


 Bertram Marsh
 7 months ago
 Views:
Transcription
1 21 st International Conference on Composite Materials Xi an, th August 2017 Numerical Modeling of Delamination Resistance Improvement Through The Use of CNTReinforced Bonding Layers Yassine ElAssami 1, Venkadesh Raman 2, Monssef DRISSIHABTI 1,3,* 1  PRES LUNAM IFSTTAR, CS4 Route de Bouaye Bouguenais, France. 2  Institut de Recherche Technologique (IRT) Jules VERNE, Chemin du Chaffault, Bouguenais, France. 3  Director of the Consortium Durability of Intelligent Composite Materials (GIS DURSI) *Corresponding Author Keywords: Composite materials, Carbon nanotubes, Homogenization, Finite elements ABSTRACT The rootsection is a high load carrying part of windturbine blade. The blade weight and stiffness properties are highly based on rootsection material properties. Weight reduction is an essential factor for blade designers to improve the energy production. So, reducing the weight by keeping the structural stiffness is important for blade. Accordingly, we have proposed Carbon NanoTube (CNT) addition in composite material for the objective of increasing the structural reinforcement in root section. CNT alignment would help to improve interlaminar property. Adding CNT in polymers which is used in composite would increase the material stiffness; to balance that we can reduce the blade weight by decreasing section thickness or number of plies. Our numerical simulation concentrates to calculate the mechanical properties of CNT contained polymer RVE (Representative volume element) model. After identifying the dispersed CNTpolymer macroscopic properties, they are applied in a macroscale model to prove their stiffness increment inbetween composite plies. 1 INTRODUCTION Carbon nanotubes (CNTs) are known for the best mechanical properties ever. Their Young's Modulus is around 5 times that of steel and their strength around 20 GPa [1] [3]. These properties make them, theoretically, the best candidates to reinforce matrix like materials. Despite their interesting properties, it is technically difficult to control their dispersion within a material. They tend to agglomerate if their concentration is high. That limits the amount of CNTs that can be added to a polymer matrix (maximum weight fraction of around 1% to 2% is usually reported in bibliography [4] [7]). Even in small amounts, it is possible to achieve noticeable improvement of the mechanical properties of a polymer. At the scale of a structure, CNTs can be applied on some specific parts to improve the resistance of some high stressed regions. In this work, polymer reinforcement with CNTs is studied at the atomic scale. We use a finite element (FEM) representative volume element (RVE) to calculate the improved properties of a CNT reinforced polymer. It is known that CNTs are very slender and their length can reach few micrometres, while their diameter is of some nanometres. In reality, their shape is usually curved. Even though this model can handle long CNTs, for practical reasons, it will be used for CNTs short enough so that the effects of curvature can be neglected. CNT atomic structure is modelled using molecular mechanics: an analogy between the CC covalent bonds and the strain energy of Euler beam elements is considered. We choose to model the atomic structure of a CNT so that some geometrical parameters such as the chirality and some defects related to functionalization [8] [10] can be controlled. As for polymers, it is more convenient to consider their engineering properties as their atomic structure is random. They are modelled as continuous media. Interaction between a CNT and the surrounding atoms of a matrix is modelled using an interface that represents the average behaviour of van der Waals interactions. No covalent interaction is considered in this model.
2 Yassine ElAssami, Venkadesh Raman and Monssef DRISSIHABTI1 In the following paper, the finite element model is briefly explained: CNT model, interface and RVE. Then, we evaluate the effect of reinforcement on the elastic properties of a nanocomposite. An application is also proposed to show the benefit of CNTs onthe improvement of resistance to shear. 2 NUMERICAL MODEL A FEM model is established to study the reinforcing effect of a CNT. The atomic structure of a CNT is simulated by a lattice of Euler beams which mechanical properties are related to the atomic of CC covalent bonds. Polymers are modelled as classical continuous media and the interface as a continuous layer linking the CNT to the reinforced matrix. 2.1 Carbon nanotube structure CNTs are allotropes of carbon of long cylindrical hollow structure. Their wall is formed by a graphenelike sheet, enrolled into a cylinder. Chirality is a geometrical that defines how the graphene sheet is enrolled. It controls the rolling direction,cc,and the diameter of the CNT. Chirality is defined with the pair (nn, mm) as follows (figure 1): CC = nnaa 1 + mmaa 2 (1) The structure of a CNT can be zigzag if m = 0, armchair if m = n or chiral in the other cases. Figure 1: Rolling direction of a graphene sheet and types of chirality The algorithm used in this work generates CNT structure based on the parameters nn, mm and a given length, by enrolling a graphene sheet. As CNT diameters used in this work are small, the fact that CNTs are not capped does not influence the results. 2.2 CNT atomic model To model a CNT in FEM, an analogy between CC bonds and Euler beam elements is used. We consider, under the hypothesis of small deformation that the energy, UU aa, for each couple of carbon atoms is equal to the elastic strain of a Euler beam, UU bb. UU aa is expressed as [9], [11]: Stretching Bending Dihedral Outofplane Van der Waals Electrostatic UU aa = UU rr + UU θθ + UU φφ + UU ωω + UU vvvvvv + UU eeee = 1 2 kk rr(δδδδ) kk θθ(δδδδ) kk ττ(δδδδ) 2 + UU vvvvvv + UU eeee (2) Stretching force constant Bending force constant Torsional constant Negligible quantities
3 21 st International Conference on Composite Materials Xi an, th August 2017 kk rr, kk θθ and kk φφ are the bond force constants of stretching, bending and torsional resistance calculated from functions of molecular mechanics [11], [12]. LL, θθ and φφ are the respectively the variations of bond length, bending and torsion angles.van der Waals effect and electrostatic forces can be neglected in front of the terms relative to the bonded interaction. UU bb is expressed as[9]: Tension energy Bending moment Torsion energy UU bb = UU AA + UU MM + UU TT = 1 EEEE 2 LL (ΔΔΔΔ) EEEE LL (ΔΔΔΔ) GGGG (3) (ΔΔΔΔ)2 LL EEandGGare the Young's and shear moduli of the beam. For a circular section, AA = ππrr 2 is the section area, II = ππrr4 ππrr4 its second moment and JJ = its polar moment. Under the hypothesis of small strain, 4 2 EE, GG and rr are constants. Considering the equality between UU aa and UU bb, we obtain: rr = 2 kk θθ, EE = kk rr 2 LL, GG = kk rr 2 kk ττ LL kk rr 4ππkk 2 θθ 8ππkk θθ (4) LL = nm is the equilibrium distance between two carbon atoms [12]. As for the bond constants, kk rr = 786 nn/nm, kk θθ = nn nm/rad 2 and νν = [13]. So, the Young's modulus of the beam elements is EE = 7753 GPa and the section radius is rr = nm. 2.2 Interface model CNT is linked to the matrix by van der Waals forces, but covalent bonds can also be forced by CNT functionalization. Covalent bonds can be modelled with the same length, and each carbon atom has only one interaction with the matrix. Van der Waals interactions are however more difficult to model as they are neither of the same length nor the same behaviour. In the present work, we consider that CNT is linked to the polymer only through van der Waals forces. The effective behaviour of the interface is modelled with a continuous layer that is different from the polymer. The thickness of this layer respects a distance of stability, h, between the CNT and polymer. The interest of using a continuous layer is that it is simple to implement and its behaviour can be controlled taking into account engineering parameters rather that atomic data. Jiang and al. [14] calculated a cohesive behaviour of the interface, based on the densities of interacting particles and atomic constants. This behaviour represents an average of the van der Waals interactions between a CNT and the reinforced polymer.
4 Yassine ElAssami, Venkadesh Raman and Monssef DRISSIHABTI1 Volume density of polymer atoms Surface density of CNT atoms LennardJones constant Bond energy at equilibrium LennardJones constant Related to equilibrium distance σσ 4 σσ cccch = 2ππ ρρ pp ρρ cc εε σσ 2 (h + vv) 4 2σσ10 5(h + vv) 10 (5) Equilibrium thickness Opening of the interface Equation (5) represents the stress σ coh as a function of the opening v of a graphene sheet in interaction with a polymer matrix. It can be used for diameters higher than that of a (n = 5, m = 5) CNT.The equilibrium distance between CNT and the polymer is h = σ. 5 Under the hypothesis of small strain, the cohesive low can be approximated by a linear behaviour of Young's modulus,ee int, with a maximum stress equal to σσ max coh where: EE int = ππρρp ρρ c εεσσ 2 (6) σσ max coh = σσ coh (σσ h) = 6ππ 5 ρρ ppρρ cc εεσσ 2 (7) For the following numerical simulations, σσ = nm, εε = nn nm and ρρ c = 4 3 3LL 2 = 38.1 nm 2 [14]. As for ρρ p, it can be estimated from the density of the polymer as the number of particles per volume unit ρρ p = 46.0 nm 3. The cohesive law calculated for shear depends on the sliding displacement, the opening and the length of CNT. Jiang and al. [14] show that shear does not vanish even though there is no sliding displacement, but its value is much smaller than the cohesive tensile stress. To account for shear in the following simulations, a Poisson's ratio equal to that of the polymer is considered. Pullout test results can for example also be used to calibrate sliding behaviour for more accuracy [15], [16]. 3 INFLUENCE OF CNT ORIENTATION Even though the mechanical properties of a CNT are very interesting, its high aspect ratio and the big difference between its stiffness and the stiffness of a polymer makes it difficult to predict the reinforced properties with classical mean field models. Morphological details are important to take into consideration. In what follows, an example is studied to show the influence of CNT orientation on the Young's modulus of a CNT reinforced polymer. CNT is oriented in different directions and its orientation relative to the loading direction is controlled by an angle α.
5 21 st International Conference on Composite Materials Xi an, th August 2017 αα LL cnt Matrix h CNT Interface LL mat Figure 2.Description of the model and example of a used mesh. The modelled CNT is armchair (10,10) (which corresponds to a diameter of 1.4 nm), with a length of 17 nm.the weight fraction is 1%. The RVE cylinder has a height of 18 nm and a diameter of 18 nm (schematic at figure 2). A short CNT has been chosen for this example so that its orientation can be varied in the range [0, 90 ] Stress [GPa] % 0.10% 0.10% Strain Neat Resin α=0 α=10 α=20 α=60 α=90 Figure 3. StrainStress curves relative to tension and compression simulations. Figure 3 shows stress strain curves, relative to tension and compression simulations for different orientations α, compared to the curve of neat matrix. Stress is calculated from the reaction force, reported to the sectional area of the cylinder. Strain is equal to the displacement of the loaded end divided by the cylinder length. As expected, stress is the highest when CNT is oriented in the load direction (α = 0 ). Stressstrain curves tend towards that of the neat resin as the orientation gets perpendicular.
6 Yassine ElAssami, Venkadesh Raman and Monssef DRISSIHABTI1 Equivalent Young Modulus E c /E mat Angle α of CNT Figure 4. Young's modulus of the composite E c as a function of the CNT orientation α. Figure 4 also shows the evolution of longitudinal Young's modulus of the composite, E c, as a function of the angle α. At α = 0, the Young's modulus is the highest: an improvement of 45% is noticed (it does not however attain the value of modulus predicted by the law of mixture as the CNT is not infinitely long). When angle α is higher, CNT participates less to load transfer until the Young's modulus reaches a plateau value at α = 40, corresponding to an improvement of less than 5%. 4 HOMOGENIZATION OF ELASTIC BEHAVIOUR The homogenization of the elastic properties of a given RVE consists in finding the relation between the macroscopic stress, σ, and macroscopic strain ε, where = 1 dv and Ω the domain Ω Ω of the RVE. However, numerical calculation of volume averages is not possible in this case, as CNT volume does not have a meaning in the present case.to encounter this problem, divergence theorem can be used to express volume averages as integrals on the outer border of the RVE Ω. An algorithm is established to calculate macroscopic fields from the boundary elements: Macroscopic stress Barycentre of the boundary facet ii Surface traction tt ii = σσ ii nn ii Area of the boundary surface ii σσ 1 ΩΩ xx ii tt ii ddss ii ii ΩΩ εε 1 2 ΩΩ (εε + εεtt ) wwheeeeee εε = nn ii uu ii ddss ii ii ΩΩ (8) Macroscopic strain Volume of domain Ω Boundary of domain Ω Unit vector normal to facet ii Displacement of facet ii Under the hypothesis of small strain, a linear relation can be considered between these two quantities, involving the macroscopic stiffness C c : σσ = C c εε (9) At small strain, the response of the material is linear elastic. In order to calculate the effective stiffness tensor, C c, of equation (9), a FEM model of a cuboid RVE has been used (figure 6). A displacement u, compatible with a macroscopic strain ε, is imposed on the border of the RVE: u = ε x, where x is the coordinate of the points of the boundary. In order to obtain the whole
7 21 st International Conference on Composite Materials Xi an, th August 2017 macroscopic stiffness tensor, compression simulations in 3 directions and shear simulations is 3 planes are needed (figure 5). Imposed displacement uu = εε xx εε = ee i ee i εε = ee i s ee j Figure 5. Schematic of boundary conditions needed to calculate the stiffness tensor. In this model, CNT is completely embedded inside the matrix. A minimum distance equal to 2h is left from the border. In order to minimize the impact of the CNT length, an important aspect ratio has been considered so that the length of the CNT is close to the length of the RVE. The CNT is armchair (6,6) with a diameter of 0.82 nm and a length of 40 nm. Matrix mesh CNT lattice Figure 6. Longitudinal cut of RVE mesh. As expected, the effective behaviour, calculated from the effective stiffness tensor C c with equation (8), is transversely isotropic, as shows table 1: EE 1 EE 3 GG νν (GPa) (GPa) 12 νν 13 GG (GPa) (GPa) Neat Polymer Matrix Nanocomposite Ratio Table 1.Homogenized properties and comparison with neat polymer matrix. The Young's modulus is doubled in the direction of the CNT with only 1% of weight fraction. The transverse Young's modulus is improved by 10%. The improvement of the elastic shear moduli is however very low. 5 RESISTANCE TO SHEAR CNTs can be used to improve some parts of the structure that are most likely to be vulnerable to some kind of loading. In what follows, an application is proposed to pointout the improvement of resistance to delamination. CNT reinforced joints can be applied between the plies to increase shear strength (figure 7).
8 Yassine ElAssami, Venkadesh Raman and Monssef DRISSIHABTI1 Shear stress Applied displacement FRP ply CNTs reinforced bonding layer Zone experiencing shear stress Fixed boundary Figure 7. Schematic of bonding layer reinforced with a CNT, experiencing shear stress. In order to evaluate the effect of CNTs in a bonding layer, we consider a cuboidal domain of polymer containing a CNT, loaded under shear. Three areas are virtually defined in this cuboid, based on the boundary conditions: an upper and a lower areas of the same size, separated by a thin area experiencing shear (figure 7). The upper and lower areas are considered as if they were inside infinitely rigid nanogrips. The boundary of the lower area is fixed and a displacement is applied on the boundary of the upper area, subjecting the middle region to shear stress. An elastoplastic model is used to account for the nonlinear behavior of the matrix. CNT orientation is controlled by angle α ( α = 0 : the CNT is parallel to shear plane. α = 90 : the CNT is perpendicular to shear plane). We follow the evolution of the resultant force applied of the upper boundary as a function of the its displacement (figure 8). The resultant force is normalized by the maximum force obtained in a simulation without CNT and the displacement is normalized by the thickness of the area under shear. As known, the neat polymer resin breaks in a brittle way once the shear strength is reached. In this case, the entire middle region reaches its maximum stress and the neat matrix separates in two independent blocks. In the case of the RVE representing the bond joint reinforced by the CNT, once shear stress is applied, the effect of nanoreinforcement can be observed. Hence, the RVE will deform in a nonlinear way. The simulations are plotted in figure 8, where a comparison is made between the cases of the neat resin versus the nanoreinforced resin with the CNT that was oriented at various directions α. Normalized Force Normalized Displacement Neat Resin α=0 α=5 α=15 α=30 α=60 α=90
9 21 st International Conference on Composite Materials Xi an, th August 2017 Figure 8. Resultant force applied on the upper boundary as a function of the boundary displacement. The resultant is normalized by maximum force of the unreinforced polymer and displacement is normalized by the middle layer thickness. The CNT strengthens the matrix by transferring a part of the applied load from upper to lower regions. It can be noticed that the strengthening effect is higher when the CNT orientation, α, is in the range 15 to 45 ; resistance to shear is provided through the C C covalent bonds. For angles lower than 15, it seems that shear is mostly resisted by the CNTpolymer interface, which explains the drop in resistance. For higher orientation angles, another drop in the resistance is noticed. This can be explained by the fact that the CNT is more efficient while under tension than under pure shear. An increase in the shear resistance up to 40% is observed. 6 CONCLUSION In order to produce high performance polymers, CNTs are very promising to attain improved mechanical properties. This improvement is stands however limited because of the difficulty to achieve a good impregnation and dispersion of CNTs when the weight fraction is high. The high aspect ratio of CNTs, their low weight fraction and their high stiffness makes it difficult to use classical methods to homogenize the mechanical behaviour. Detailed models are needed to take into account the high anisotropy. Indeed, the model used here shows a big influence of some morphological details such as CNT orientation. As the control of CNTs orientation is technically difficult to achieve industrially, the mechanical behaviour is not optimal in the reality. But the loss of elastic stiffness due to the random dispersion of CNTs is outbalanced by the improvement of other resistance mechanisms, such as shear strength, as emphasized in the last simulations. One of the advantages of the model that was developed is that it is suitable to handle CNTs of sizes that are industrially available (lengths in the range nm were used in current simulations). It is also possible to consider local defects on the CNT atomic lattice, due to functionalization for example, as well as stronger bonds on the interface. 7 REFERENCES [1] R. S. Ruoff, D. Qian, and W. K. Liu, Mechanical properties of carbon nanotubes: theoretical predictions and experimental measurements, Comptes Rendus Phys., vol. 4, no. 9, pp , Nov [2] M. Meo and M. Rossi, Prediction of Young s modulus of single wall carbon nanotubes by molecularmechanics based finite element modelling, Compos. Sci. Technol., vol. 66, no , pp , Sep [3] K. I. Tserpes, P. Papanikos, and S. A. Tsirkas, A progressive fracture model for carbon nanotubes, Compos. Part B Eng., vol. 37, no. 7 8, pp , Oct [4] D. Qian, E. C. Dickey, R. Andrews, and T. Rantell, Load transfer and deformation mechanisms in carbon nanotubepolystyrene composites, Appl. Phys. Lett., vol. 76, no. 20, pp , May [5] B. Fiedler, F. H. Gojny, M. H. G. Wichmann, M. C. M. Nolte, and K. Schulte, Fundamental aspects of nanoreinforced composites, Compos. Sci. Technol., vol. 66, no. 16, pp , Dec [6] A. Montazeri and N. Montazeri, Viscoelastic and mechanical properties of multi walled carbon nanotube/epoxy composites with different nanotube content, Mater. Des., vol. 32, no. 4, pp , Apr [7] F. Vahedi, H. R. Shahverdi, M. M. Shokrieh, and M. Esmkhani, Effects of carbon nanotube content on the mechanical and electrical properties of epoxybased composites, New Carbon Mater., vol. 29, no. 6, pp , Dec
10 Yassine ElAssami, Venkadesh Raman and Monssef DRISSIHABTI1 [8] G. M. Odegard, T. S. Gates, L. M. Nicholson, and K. E. Wise, Equivalentcontinuum modeling of nanostructured materials, Compos. Sci. Technol., vol. 62, no. 14, pp , Nov [9] C. Li and T.W. Chou, A structural mechanics approach for the analysis of carbon nanotubes, Int. J. Solids Struct., vol. 40, no. 10, pp , May [10] C. Li and T.W. Chou, Multiscale Modeling of Carbon Nanotube Reinforced Polymer Composites, J. Nanosci. Nanotechnol., vol. 3, no. 5, pp , [11] A. K. Rappe, C. J. Casewit, K. S. Colwell, W. A. Goddard, and W. M. Skiff, UFF, a full periodic table force field for molecular mechanics and molecular dynamics simulations, J. Am. Chem. Soc., vol. 114, no. 25, pp , Dec [12] D. W. Brenner, O. A. Shenderova, J. A. Harrison, S. J. Stuart, B. Ni, and S. B. Sinnott, A secondgeneration reactive empirical bond order (REBO) energy expression for hydrocarbons, J. Phys. Condens. Matter, vol. 14, no. 4, p. 783, [13] X. Lu and Z. Hu, Mechanical property evaluation of singlewalled carbon nanotubes by finite element modeling, Compos. Part B Eng., vol. 43, no. 4, pp , Jun [14] L. Y. Jiang et al., A cohesive law for carbon nanotube/polymer interfaces based on the van der Waals force, J. Mech. Phys. Solids, vol. 54, no. 11, pp , Nov [15] S. Namilae and N. Chandra, Multiscale Model to Study the Effect of Interfaces in Carbon NanotubeBased Composites, J. Eng. Mater. Technol., vol. 127, no. 2, pp , Apr [16] Y. L. Chen, B. Liu, X. Q. He, Y. Huang, and K. C. Hwang, Failure analysis and the optimal toughness design of carbon nanotubereinforced composites, Compos. Sci. Technol., vol. 70, no. 9, pp , Sep
Nonlinear Mechanics of Monolayer Graphene Rui Huang
Nonlinear Mechanics of Monolayer Graphene Rui Huang Center for Mechanics of Solids, Structures and Materials Department of Aerospace Engineering and Engineering Mechanics The University of Texas at Austin
More informationGraduate School of Engineering, Kyoto University, Kyoto daigakukatsura, Nishikyoku, Kyoto, Japan.
On relationship between contact surface rigidity and harmonic generation behavior in composite materials with mechanical nonlinearity at fibermatrix interface (Singapore November 2017) N. Matsuda, K.
More informationNonlocal material properties of single walled carbon nanotubes
Nonlocal material properties of single walled carbon nanotubes J. V. Araújo dos Santos * and C. M. Mota Soares IDMEC, Instituto Superior Técnico, Universidade Técnica de Lisboa, Portugal Av. Rovisco Pais,
More informationIntensity (a.u.) Intensity (a.u.) Raman Shift (cm 1 ) Oxygen plasma. 6 cm. 9 cm. 1mm. Singlelayer graphene sheet. 10mm. 14 cm
Intensity (a.u.) Intensity (a.u.) a Oxygen plasma b 6 cm 1mm 10mm Singlelayer graphene sheet 14 cm 9 cm Flipped Si/SiO 2 Patterned chip Plasmacleaned glass slides c d After 1 sec normal Oxygen plasma
More informationCHARACTERIZING MECHANICAL PROPERTIES OF GRAPHITE USING MOLECULAR DYNAMICS SIMULATION
CHARACTERIZING MECHANICAL PROPERTIES OF GRAPHITE USING MOLECULAR DYNAMICS SIMULATION JiaLin Tsai and JieFeng Tu Department of Mechanical Engineering, National Chiao Tung University 1001 University Road,
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationThe Young s Modulus of SingleWalled Carbon Nanotubes
The Young s Modulus of SingleWalled Carbon Nanotubes Douglas Vodnik Faculty Advisor: Dr. Kevin Crosby Department of Physics, Carthage College, Kenosha, WI Abstract A new numerical method for calculating
More informationAngular Momentum, Electromagnetic Waves
Angular Momentum, Electromagnetic Waves Lecture33: Electromagnetic Theory Professor D. K. Ghosh, Physics Department, I.I.T., Bombay As before, we keep in view the four Maxwell s equations for all our discussions.
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationDefense Technical Information Center Compilation Part Notice
UNCLASSIFIED Defense Technical Information Center Compilation Part Notice ADP012151 TITLE: Chemical Bonding of Polymer on Carbon Nanotube DISTRIBUTION: Approved for public release, distribution unlimited
More informationMATERIALS. Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle?
MATERIALS Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: A. Composition
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More information**********************************************************************
Department of Civil and Environmental Engineering School of Mining and Petroleum Engineering 333 Markin/CNRL Natural Resources Engineering Facility www.engineering.ualberta.ca/civil Tel: 780.492.4235
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationAnalysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements
Acta Mech. Sin. (2016) 32(2):295 300 DOI 10.1007/s1040901505342 RESEARCH PAPER Analysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements V. H. Carneiro 1
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationMechanical Behavior of Fullerene Reinforced Fiber Composites with Interface Defects through Homogenization Approach and Finite Element Method
, pp.6782 http://dx.doi.org/1.14257/ijast.215.78.6 Mechanical Behavior of Fullerene Reinforced Fiber Composites with Interface Defects through Homogenization Approach and Finite Element Method P. Prasanthi
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationApplication to modeling brittle materials
1.01, 3.01, 10.333,.00 Introduction to Modeling and Simulation Spring 011 Part I Continuum and particle methods Application to modeling brittle materials Lecture 7 Markus J. Buehler Laboratory for Atomistic
More informationON CALCULATION OF EFFECTIVE ELASTIC PROPERTIES OF MATERIALS WITH CRACKS
Materials Physics and Mechanics 32 (2017) 213221 Received: November 7, 2017 ON CALCULATION OF EFFECTIVE ELASTIC PROPERTIES OF MATERIALS WITH CRACKS Ruslan L. Lapin 1, Vitaly A. Kuzkin 1,2 1 Peter the
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationThe peeling behavior of thin films with finite bending sti ness and the implications on gecko adhesion
The peeling behavior of thin films with finite bending sti ness and the implications on gecko adhesion Roger A. Sauer 1 Aachen Institute for Advanced Study in Computational Engineering Science (AICES),
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationLOADING MODE DEPENDENT EFFECTIVE PROPERTIES OF OCTETTRUSS LATTICE STRUCTURES USING 3DPRINTING. Adithya C hallapalli
LOADING MODE DEPENDENT EFFECTIVE PROPERTIES OF OCTETTRUSS LATTICE STRUCTURES USING 3DPRINTING Adithya C hallapalli Thesis Prepared for the Degree of MASTER OF SCIENCE UNIVERSITY OF NORTH TEXAS May 215
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationGame Physics. Game and Media Technology Master Program  Utrecht University. Dr. Nicolas Pronost
Game and Media Technology Master Program  Utrecht University Dr. Nicolas Pronost Soft body physics Soft bodies In reality, objects are not purely rigid for some it is a good approximation but if you hit
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationANALYSIS AND NUMERICAL MODELLING OF CERAMIC PIEZOELECTRIC BEAM BEHAVIOR UNDER THE EFFECT OF EXTERNAL SOLICITATIONS
Third International Conference on Energy, Materials, Applied Energetics and Pollution. ICEMAEP016, October 3031, 016, Constantine,Algeria. ANALYSIS AND NUMERICAL MODELLING OF CERAMIC PIEZOELECTRIC BEAM
More informationFIXED BEAMS IN BENDING
FIXED BEAMS IN BENDING INTRODUCTION Fixed or builtin beams are commonly used in building construction because they possess high rigidity in comparison to simply supported beams. When a simply supported
More informationTransactions on Engineering Sciences vol 14, 1997 WIT Press, ISSN
On the Computation of Elastic Elastic Rolling Contact using Adaptive Finite Element Techniques B. Zastrau^, U. Nackenhorst*,J. Jarewski^ ^Institute of Mechanics and Informatics, Technical University Dresden,
More informationLecture 7, Foams, 3.054
Lecture 7, Foams, 3.054 Opencell foams StressStrain curve: deformation and failure mechanisms Compression  3 regimes  linear elastic  bending  stress plateau  cell collapse by buckling yielding
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More information3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationAim of the study Experimental determination of mechanical parameters Local buckling (wrinkling) Failure maps Optimization of sandwich panels
METNET Workshop October 1112, 2009, Poznań, Poland Experimental and numerical analysis of sandwich metal panels Zbigniew Pozorski, Monika ChudaKowalska, Robert Studziński, Andrzej Garstecki Poznan University
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationCHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationMechanics of Irregular Honeycomb Structures
Mechanics of Irregular Honeycomb Structures S. Adhikari 1, T. Mukhopadhyay 1 Chair of Aerospace Engineering, College of Engineering, Swansea University, Singleton Park, Swansea SA2 8PP, UK Sixth International
More informationMechanical Design in Optical Engineering
OPTI Buckling Buckling and Stability: As we learned in the previous lectures, structures may fail in a variety of ways, depending on the materials, load and support conditions. We had two primary concerns:
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationCoulomb s Law and Coulomb s Constant
PreLab Quiz / PHYS 224 Coulomb s Law and Coulomb s Constant Your Name: Lab Section: 1. What will you investigate in this lab? 2. Consider a capacitor created when two identical conducting plates are placed
More informationFermi Surfaces and their Geometries
Fermi Surfaces and their Geometries Didier Ndengeyintwali Physics Department, Drexel University, Philadelphia, Pennsylvania 19104, USA (Dated: May 17, 2010) 1. Introduction The Pauli exclusion principle
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationFinite Element Modeling of an Aluminum Tricycle Frame
Finite Element Modeling of an Aluminum Tricycle Frame A. Rodríguez, B. Chiné*, and J. A. Ramírez Costa Rica Institute of Technology, School of Materials Science and Engineering, Cartago, Costa Rica *Corresponding
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationAspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites
Aspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites J.A.Nairn Wood Science and Engineering, Oregon State University, Corvallis, OR 97330, USA Abstract A fiber s efficiency in a
More informationGeometrydependent MITC method for a 2node isobeam element
Structural Engineering and Mechanics, Vol. 9, No. (8) 33 Geometrydependent MITC method for a node isobeam element PhillSeung Lee Samsung Heavy Industries, Seocho, Seoul 37857, Korea HyuChun Noh
More informationContinuum modeling of van der Waals interactions between. carbon nanotube walls
Contuum modelg of van der Waals teractions between carbon nanotube walls W.B. Lu 1, B. Liu 1a), J. Wu 1, J. Xiao, K.C. Hwang 1, S. Y. Fu 3,4 a), Y. Huang 1 FML, Department of Engeerg Mechanics, Tsghua
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More informationAnalysis of high loss viscoelastic composites
Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science
More informationA multiscale approach for composite materials as multifield continua
Materials Science Forum Vols. 539543 (27) pp. 25512556 online at http://www.scientific.net (27) Trans Tech Publications, Switzerland A multiscale approach for composite materials as multifield continua
More informationBrittle Deformation. Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm
Lecture 6 Brittle Deformation Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm WW Norton, unless noted otherwise Brittle deformation EarthStructure (2 nd
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationDETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1
PERIODICA POLYTECHNICA SER. CIV. ENG. VOL. 46, NO. 1, PP. 125 148 (2002) DETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1 Nándor LIEGNER Department of Highway and Railway Engineering
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationAnalysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method
Analysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method V.M.F. Nascimento Departameto de ngenharia Mecânica TM, UFF, Rio de Janeiro
More informationRVE Analysis of Light Weight Carbon Nanotubes Embedded Piezoelectric Fibre Composites
Nanoscience and Nanotechnology 2016, 6(1): 1116 DOI: 10.5923/j.nn.20160601.03 RVE Analysis of Light Weight Carbon Nanotubes Embedded Piezoelectric Fibre Composites V. K. Srivastava 1,*, H. Berger 2, U.
More informationParametric analysis and torsion design charts for axially restrained RC beams
Structural Engineering and Mechanics, Vol. 55, No. 1 (2015) 127 DOI: http://dx.doi.org/10.12989/sem.2015.55.1.001 1 Parametric analysis and torsion design charts for axially restrained RC beams Luís F.A.
More informationLINEAR AND NONLINEAR SHELL THEORY. Contents
LINEAR AND NONLINEAR SHELL THEORY Contents Straindisplacement relations for nonlinear shell theory Approximate straindisplacement relations: Linear theory Small strain theory Small strains & moderate
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More informationDegree Thesis Flexural Rigidity (D) in Beams. Author: Zious Karis. Instructor: Rene Herrmann
Degree Thesis Flexural Rigidity (D) in Beams Author: Zious Karis Instructor: Rene Herrmann Degree Thesis Materials Processing Technology 2017 DEGREE THESIS Arcada University of Applied Sciences, Helsinki,
More informationA Piezoelectric Screw Dislocation Interacting with an Elliptical Piezoelectric Inhomogeneity Containing a Confocal Elliptical Rigid Core
Commun. Theor. Phys. 56 774 778 Vol. 56, No. 4, October 5, A Piezoelectric Screw Dislocation Interacting with an Elliptical Piezoelectric Inhomogeneity Containing a Confocal Elliptical Rigid Core JIANG
More informationBending Analysis of a Cantilever Nanobeam With End Forces by Laplace Transform
International Journal of Engineering & Applied Sciences (IJEAS) Vol.9, Issue (Special Issue: Composite Structures) (07) 03 http://.doi.org/0.407/ijeas.34635 Int J Eng Appl Sci 9() (07) 03 Bending Analysis
More information*MAT_PAPER  a new orthotropic elastoplastic model for paper materials
*MAT_PAPER  a new orthotropic elastoplastic model for paper materials Jesper Karlsson, Dynamore Nordic Mikael Schill, Dynamore Nordic Johan Tryding, Tetra Pak *MAT_PAPER (*MAT_274) A new orthotropic elastoplastic
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationMultiscale mechanics and structure of semihard cheese
Multiscale mechanics and structure of semihard cheese T.J. Faber a,b, P.J.Schreurs b, J.M.J.G. Luyten a, H.E.H.Meijer b a FrieslandCampina Research, Deventer, The Netherlands (timo.faber@frieslandcampina.com))
More informationSchur decomposition in the scaled boundary finite element method in elastostatics
IOP Conference Series: Materials Science and Engineering Schur decomposition in the scaled boundary finite element method in elastostatics o cite this article: M Li et al 010 IOP Conf. Ser.: Mater. Sci.
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationUnit III Theory of columns. Dr.P.Venkateswara Rao, Associate Professor, Dept. of Civil Engg., SVCE, Sriperumbudir
Unit III Theory of columns 1 Unit III Theory of Columns References: Punmia B.C.,"Theory of Structures" (SMTS) Vol II, Laxmi Publishing Pvt Ltd, New Delhi 2004. Rattan.S.S., "Strength of Materials", Tata
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More informationMultiscale modeling of failure in ABS materials
Institute of Mechanics Multiscale modeling of failure in ABS materials Martin Helbig, Thomas Seelig 15. International Conference on Deformation, Yield and Fracture of Polymers Kerkrade, April 2012 Institute
More informationMOLECULAR MODELLING OF STRESSES AND DEFORMATIONS IN NANOSTRUCTURED MATERIALS
Int. J. Appl. Math. Comput. Sci., 2004, Vol. 14, No. 4, 541 548 MOLECULAR MODELLING OF STRESSES AND DEFORMATIONS IN NANOSTRUCTURED MATERIALS GWIDON SZEFER Institute of Structural Mechanics, AGH University
More informationA General Equation for Fitting Contact Area and Friction vs Load Measurements
Journal of Colloid and Interface Science 211, 395 400 (1999) Article ID jcis.1998.6027, available online at http://www.idealibrary.com on A General Equation for Fitting Contact Area and Friction vs Load
More informationReference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity",
Reference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity", Oxford University Press, Oxford. J. Lubliner, "Plasticity
More informationInternal lattice relaxation of singlelayer graphene under inplane deformation. Jun Zhou and Rui Huang
Internal lattice relaxation of singlelayer graphene under inplane deformation Jun Zhou and Rui Huang Department of Aerospace Engineering and Engineering Mechanics, University of Texas, Austin, TX 7871
More information